# Rewrite the expression for the total free energy change for nucleation

14:440:407 ch10
Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for
the case of a cubic nucleus of edge length a (instead of a sphere of radius r). Now differentiate this expression
with respect to a (per Equation 10.2) and solve for both the critical cube edge length, a*, and also ΔG*.
(b) Is ΔG* greater for a cube or a sphere? Why?
Solution:
(a) This problem first asks that we rewrite the expression for the total free energy change for nucleation
(analogous to Equation 10.1) for the case of a cubic nucleus of edge length a. The volume of such a cubic radius is
a3, whereas the total surface area is 6a2 (since there are six faces each of which has an area of a2). Thus, the
expression for ΔG is as follows:
ΔG = a 3ΔGv + 6a 2 γ
Differentiation of this expression with respect to a is as
d (a 3ΔGv ) d (6a 2 γ)
d ΔG
=
+
da
da
da
= 3a 2 ΔGv + 12a γ
If we set this expression equal to zero as
3a 2 ΔGv + 12a γ = 0
and then solve for a (= a*), we have
a* = −
4γ
ΔGv
Substitution of this expression for a in the above expression for ΔG yields an equation for ΔG* as
ΔG * = (a*) 3 ΔGv + 6(a*) 2 γ
⎛ 4 γ ⎞3
⎛ 4 γ ⎞2
⎟⎟ ΔGv + 6 γ ⎜⎜−
⎟⎟
= ⎜⎜−
⎝ ΔGv ⎠
⎝ ΔGv ⎠
=
32 γ 3
(ΔGv ) 2
⎡
⎤
⎛ 16 π ⎞⎡ γ 3 ⎤
γ3 ⎥
⎥ =
ΔGv for a cube—i.e., (32) ⎢
—is greater that for a sphere—i.e., ⎜
⎟⎢
⎝ 3 ⎠⎢⎣ (ΔG ) 2 ⎥⎦
⎢⎣ (ΔG ) 2 ⎥⎦
v
v
⎡
⎤
γ3 ⎥
. The reason for this is that surface-to-volume ratio of a cube is greater than for a sphere.
(16.8) ⎢
⎢⎣ (ΔG ) 2 ⎥⎦
v
(b)
Question 10.3: If copper (which has a melting point of 1085&deg;C) homogeneously nucleates at 849&deg;C, calculate
the critical radius given values of –1.77 &times; 109 J/m3 and 0.200 J/m2, respectively, for the latent heat of fusion
and the surface free energy.
Solution:
This problem states that copper homogeneously nucleates at 849&deg;C, and that we are to calculate the critical
radius given the latent heat of fusion (–1.77 &times; 109 J/m3) and the surface free energy (0.200 J/m2). Solution to this
problem requires the utilization of Equation 10.6 as
⎛ 2 γT ⎞ ⎛
⎞
m ⎟⎜ 1
⎟
r * = ⎜−
⎜ ΔH ⎟ ⎜⎝ T − T ⎟⎠
f ⎠ m
⎝
⎡ (2)(0.200 J / m2 ) (1085 + 273 K) ⎤ ⎛
⎞
1
= ⎢−
⎥
⎜
⎟
−1.77 &times; 10 9 J / m3
⎣
⎦ ⎝ 1085&deg;C − 849&deg;C ⎠
= 1.30 &times; 10−9 m = 1.30 nm
Question 10.4: (a) For the solidification of iron, calculate the critical radius r* and the activation free energy
ΔG* if nucleation is homogeneous. Values for the latent heat of fusion and surface free energy are –1.85 &times; 109
J/m3 and 0.204 J/m2, respectively. Use the supercooling value found in Table 10.1.
(b) Now calculate the number of atoms found in a nucleus of critical size. Assume a lattice parameter
of 0.292 nm for solid iron at its melting temperature.
Solution:
(a) This portion of the problem asks that we compute r* and ΔG* for the homogeneous nucleation of the
solidification of Fe. First of all, Equation 10.6 is used to compute the critical radius. The melting temperature for
iron, found inside the front cover is 1538&deg;C; also values of ΔHf (–1.85 &times; 109 J/m3) and γ (0.204 J/m2) are given in
the problem statement, and the supercooling value found in Table 10.1 is 295&deg;C (or 295 K). Thus, from Equation
10.6 we have
⎛ 2γT ⎞ ⎛
1 ⎞
m ⎟⎜
r * = ⎜−
⎜ ΔH ⎟ ⎜ T − T ⎟⎟
⎠
f ⎠⎝ m
⎝
⎡ (2) (0.204 J / m2 ) (1538 + 273 K) ⎤ ⎛ 1 ⎞
= ⎢−
⎥⎜
⎟
−1.85 &times; 10 9 J / m 3
⎣
⎦ ⎝ 295 K ⎠
= 1.35 &times; 10−9 m = 1.35 nm
For computation of the activation free energy, Equation 10.7 is employed. Thus
⎛
⎞
1
16 π γ 3Tm2 ⎟
ΔG * = ⎜
⎜ 3 ΔH 2 ⎟ (T − T ) 2
f ⎠ m
⎝
3
⎡
⎤
⎤
1
(16)(π) ( 0.204 J / m 2 ) (1538 + 273 K) 2 ⎥⎡
=⎢
⎢
⎥
2
2
⎢⎣
⎥⎦⎣ (295 K) ⎦
(3) (−1.85 &times; 10 9 J / m3 )
= 1.57 &times; 10−18 J
(b) In order to compute the number of atoms in a nucleus of critical size (assuming a spherical nucleus of
radius r*), it is first necessary to determine the number of unit cells, which we then multiply by the number of atoms
per unit cell. The number of unit cells found in this critical nucleus is just the ratio of critical nucleus and unit cell
volumes. Inasmuch as iron has the BCC crystal structure, its unit cell volume is just a3 where a is the unit cell
length (i.e., the lattice parameter); this value is 0.292 nm, as cited in the problem statement. Therefore, the number
of unit cells found in a radius of critical size is just
4
πr * 3
3
# unit cells / particle =
a3
=
⎛4⎞
⎜ ⎟ (π)(1.35
⎝ 3⎠
nm) 3
(0.292 nm) 3
= 414 unit cells
Inasmuch as 2 atoms are associated with each BCC unit cell, the total number of atoms per critical nucleus is just
(414 unit cells / critical nucleus)(2 atoms / unit cell) = 828 atoms / critical nucleus
Question 10.5: (a) Assume for the solidification of iron (Problem 10.4) that nucleation is homogeneous, and
the number of stable nuclei is 106 nuclei per cubic meter. Calculate the critical radius and the number of
stable nuclei that exist at the following degrees of supercooling: 200 K and 300 K.
(b) What is significant about the magnitudes of these critical radii and the numbers of stable nuclei?
Solution:
(a) For this part of the problem we are asked to calculate the critical radius for the solidification of iron
(per Problem 10.4), for 200 K and 300 K degrees of supercooling, and assuming that the there are 106 nuclei per
meter cubed for homogeneous nucleation. In order to calculate the critical radii, we replace the Tm – T term in
Equation 10.6 by the degree of supercooling (denoted as ΔT) cited in the problem.
For 200 K supercooling,
⎛
⎞
* = ⎜− 2 γTm ⎟ ⎛⎜ 1 ⎞⎟
r200
⎜ ΔH ⎟ ⎝ ΔT ⎠
f ⎠
⎝
⎡ (2)(0.204 J / m2 ) (1538 + 273 K) ⎤ ⎛ 1 ⎞
= ⎢−
⎥⎜
⎟
−1.85 &times; 10 9 J / m 3
⎣
⎦ ⎝ 200 K ⎠
= 2.00 &times; 10-9 m = 2.00 nm
And, for 300 K supercooling,
2
⎡
⎤⎛
⎞
* = ⎢− (2)(0.204 J / m ) (1538 + 273 K) ⎥ ⎜ 1 ⎟
r300
9
3
−1.85 &times; 10 J / m
⎣
⎦ ⎝ 300 K ⎠
= 1.33 &times; 10-9 m = 1.33 nm
In order to compute the number of stable nuclei that exist at 200 K and 300 K degrees of supercooling, it is
necessary to use Equation 10.8. However, we must first determine the value of K1 in Equation 10.8, which in turn
requires that we calculate ΔG* at the homogeneous nucleation temperature using Equation 10.7; this was done in
Problem 10.4, and yielded a value of ΔG* = 1.57 &times; 10-18 J. Now for the computation of K1, using the value of n*
for at the homogenous nucleation temperature (106 nuclei/m3):
K1 =
n*
⎛ ΔG * ⎞
exp ⎜−
⎟
⎝ kT ⎠
=
10 6 nuclei / m3
⎡
⎤
1.57 &times; 10−18 J
exp ⎢−
⎥
−23
⎣ (1.38 &times; 10 J / atom − K) (1538&deg;C − 295&deg;C) ⎦
= 5.62 &times; 1045 nuclei/m3
Now for 200 K supercooling, it is first necessary to recalculate the value ΔG* of using Equation 10.7, where, again,
the Tm – T term is replaced by the number of degrees of supercooling, denoted as ΔT, which in this case is 200 K.
Thus
⎛
3 2⎞
* = ⎜ 16 π γ Tm ⎟ 1
ΔG200
⎜ 3 ΔH 2 ⎟ (ΔT ) 2
f ⎠
⎝
⎡ (16)(π) (0.204 J / m 2 )3 (1538 + 273 K) 2 ⎤⎡
⎤
1
=⎢
⎥
⎥⎢
9
3
2
2
(3)(−1.85 &times; 10 J / m )
⎣
⎦⎣ (200 K) ⎦
= 3.41 &times; 10-18 J
And, from Equation 10.8, the value of n* is
⎛
* ⎞
* = K exp ⎜− ΔG200 ⎟
n200
1
⎜
kT ⎟⎠
⎝
⎡
⎤
3.41 &times; 10−18 J
= (5.62 &times; 10 45 nuclei / m3) exp ⎢−
⎥
−
23
⎣ (1.38 &times; 10 J / atom − K) (1538 K − 200 K) ⎦
= 3.5 &times; 10-35 stable nuclei
Now, for 300 K supercooling the value of ΔG* is equal to
2 3
2 ⎤⎡
⎡
⎤
1
* = ⎢ (16)(π) (0.204 J / m ) (1538 + 273 K) ⎥⎢
ΔG300
⎥
9
3
2
2
(3)(−1.85 &times; 10 J / m )
⎣
⎦⎣ (300 K) ⎦
= 1.51 &times; 10-18 J
from which we compute the number of stable nuclei at 300 K of supercooling as
⎛
* ⎞
* = K exp ⎜− ΔG300 ⎟
n300
1
⎜
kT ⎟⎠
⎝
⎡
⎤
1.51 &times; 10−18 J
n* = (5.62 &times; 10 45 nuclei / m3) exp ⎢−
⎥
−
23
⎣ (1.38 &times; 10 J / atom − K) (1538 K − 300 K) ⎦
= 2.32 &times; 107 stable nuclei
(b) Relative to critical radius, r* for 300 K supercooling is slightly smaller that for 200 K (1.33 nm versus
2.00 nm). [From Problem 10.4, the value of r* at the homogeneous nucleation temperature (295 K) was 1.35 nm.]
More significant, however, are the values of n* at these two degrees of supercooling, which are dramatically
different—3.5 &times; 10-35 stable nuclei at ΔT = 200 K, versus 2.32 &times; 107 stable nuclei at ΔT = 300 K!
Question 10.6: For some transformation having kinetics that obey the Avrami equation (Equation 10.17), the
parameter n is known to have a value of 1.7. If, after 100 s, the reaction is 50% complete, how long (total
time) will it take the transformation to go to 99% completion?
Solution:
This problem calls for us to compute the length of time required for a reaction to go to 99% completion. It
first becomes necessary to solve for the parameter k in Equation 10.17. In order to do this it is best manipulate the
equation such that k is the dependent variable. We first rearrange Equation 10.17 as
exp (− kt n ) = 1 − y
and then take natural logarithms of both sides:
− kt n = ln (1 − y)
Now solving for k gives
k =−
ln (1 − y)
tn
And, from the problem statement, for y = 0.50 when t = 100 s and given that n = 1.7, the value of k is equal to
k =−
ln (1 − 0.5)
= 2.76 &times; 10 -4
(100 s)1.7
We now want to manipulate Equation 10.17 such that t is the dependent variable. The above equation may be
written in the form:
tn = −
ln (1 − y)
k
And solving this expression for t leads to
⎡ ln (1 − y ) ⎤
t = ⎢−
⎥⎦
⎣
k
1/n
Now, using this equation and the value of k determined above, the time to 99% transformation completion is equal
to
⎡ ln (1 − 0.99) ⎤1/1.7
= 305 s
t = ⎢−
⎥
⎣ 2.76 &times; 10−4 ⎦
Question 10.8: It is known that the kinetics of recrystallization for some alloy obey the Avrami equation and
that the value of n in the exponential is 2.5. If, at some temperature, the fraction recrystallized is 0.40 after
200 min, determine the rate of recrystallization at this temperature.
Solution:
This problem gives us the value of y (0.40) at some time t (200 min), and also the value of n (2.5) for the
recrystallization of an alloy at some temperature, and then asks that we determine the rate of recrystallization at this
same temperature. It is first necessary to calculate the value of k. We first rearrange Equation 10.17 as
exp (− kt n ) = 1 −
y
and then take natural logarithms of both sides:
− kt n = ln (1 − y)
Now solving for k gives
k =−
ln (1 − y)
tn
which, using the values cited above for y, n, and t yields
k =−
ln (1 − 0.40)
= 9.0 &times; 10 -7
(200 min) 2.5
At this point we want to compute t0.5, the value of t for y = 0.5, which means that it is necessary to establish a form
of Equation 10.17 in which t is the dependent variable. From one of the above equations
tn = −
And solving this expression for t leads to
ln (1 − y)
k
⎡ ln (1 − y) ⎤1/n
t = ⎢−
⎥⎦
⎣
k
For t0.5, this equation takes the form
⎡ ln (1 − 0.5) ⎤1/ n
t0.5 = ⎢−
⎥⎦
⎣
k
and incorporation of the value of k determined above, as well as the value of n cited in the problem statement (2.5),
then t0.5 is equal to
⎡ ln (1 − 0.5) ⎤1/2.5
= 226.3 min
t0.5 = ⎢−
⎥
⎣ 9.0 &times; 10−7 ⎦
Therefore, from Equation 10.18, the rate is just
rate =
1
t0.5
=
1
= 4.42 &times; 10 -3 (min) -1
226.3 min
Question 10.9: The kinetics of the austenite-to-pearlite transformation obey the Avrami relationship. Using
the fraction transformed–time data given here, determine the total time required for 95% of the austenite to
transform to pearlite:
Fraction Transformed
Time (s)
0.2
12.6
0.8
28.2
Solution:
The first thing necessary is to set up two expressions of the form of Equation 10.17, and then to solve
simultaneously for the values of n and k. In order to expedite this process, we will rearrange and do some algebraic
manipulation of Equation 10.17. First of all, we rearrange as follows:
( )
1 − y = exp − kt n
Now taking natural logarithms
ln (1 − y) = − kt n
Or
− ln (1 − y) = kt n
which may also be expressed as
⎛ 1 ⎞
ln ⎜
⎟ = kt n
⎝1 − y ⎠
Now taking natural logarithms again, leads to
⎡ ⎛ 1
ln ⎢ ln ⎜
⎣ ⎝1 −
⎞⎤
⎟⎥ = ln k + n ln t
y ⎠⎦
which is the form of the equation that we will now use. Using values cited in the problem statement, the two
equations are thus
⎧ ⎡ 1 ⎤⎫
ln ⎨ ln ⎢
⎥⎬ = ln k + n ln (12.6 s)
⎩ ⎣ 1 − 0.2 ⎦⎭
⎧ ⎡ 1 ⎤⎫
ln ⎨ ln ⎢
⎥⎬ = ln k + n ln (28.2 s)
⎩ ⎣ 1 − 0.8 ⎦⎭
Solving these two expressions simultaneously for n and k yields n = 2.453 and k = 4.46 &times; 10-4.
Now it becomes necessary to solve for the value of t at which y = 0.95. One of the above equations—viz
− ln (1 − y) = kt n
may be rewritten as
tn = −
ln (1 − y)
k
And solving for t leads to
⎡ ln (1 − y) ⎤1/n
t = ⎢−
⎥⎦
⎣
k
Now incorporating into this expression values for n and k determined above, the time required for 95% austenite
transformation is equal to
⎡ ln (1 − 0.95) ⎤1/2.453
= 35.7 s
t = ⎢−
⎥
⎣ 4.64 &times; 10−4 ⎦
Question 10.11: (a) From the curves shown in Figure 10.11 and using Equation 10.18, determine the rate of
recrystallization for pure copper at the several temperatures.
(b) Make a plot of ln(rate) versus the reciprocal of temperature (in K–1), and determine the activation
energy for this recrystallization process. (See Section 5.5.)
(c) By extrapolation, estimate the length of time required for 50% recrystallization at room
temperature, 20&deg;C (293 K).
Solution:
This problem asks us to consider the percent recrystallized versus logarithm of time curves for copper
shown in Figure 10.11.
(a) The rates at the different temperatures are determined using Equation 10.18, which rates are tabulated
below:
Temperature (&deg;C)
Rate (min)-1
135
0.105
119
4.4 &times; 10-2
113
2.9 &times; 10-2
102
1.25 &times; 10-2
88
4.2 &times; 10-3
43
3.8 &times; 10-5
(b) These data are plotted below.
The activation energy, Q, is related to the slope of the line drawn through the data points as
Q = − Slope (R)
where R is the gas constant. The slope of this line is equal to
Slope =
Δ ln rate
ln rate1 − ln rate 2
=
⎛1⎞
1
1
−
Δ⎜ ⎟
T1
T2
⎝T ⎠
Let us take 1/T1 = 0.0025 K-1 and 1/T2 = 0.0031 K-1; the corresponding ln rate values are ln rate1 = -2.6 and ln
rate2 = -9.4. Thus, using these values, the slope is equal to
Slope =
−2.6 − (−9.4)
= − 1.133 &times; 10 4 K
0.0025 K -1 − 0.0031 K -1
And, finally the activation energy is
Q = − (Slope)(R) = − (−1.133 &times; 10 4 K -1 ) (8.31 J/mol - K)
= 94,150 J/mol
(c) At room temperature (20&deg;C), 1/T = 1/(20 + 273 K) = 3.41 &times; 10-3 K-1. Extrapolation of the data in the
plot to this 1/T value gives
ln (rate) ≅ − 12.8
rate ≅ exp (−12.8) = 2.76 &times; 10 -6 (min) -1
But since
rate =
t0.5 =
1
t0.5
1
1
=
rate 2.76 &times; 10−6 (min)−1
= 3.62 &times; 10 5 min = 250 days
Question 10.14: (a) Briefly describe the phenomena of superheating and supercooling.
(b) Why do these phenomena occur?
Solution:
(a) Superheating and supercooling correspond, respectively, to heating or cooling above or below a phase
transition temperature without the occurrence of the transformation.
(b) These phenomena occur because right at the phase transition temperature, the driving force is not
sufficient to cause the transformation to occur. The driving force is enhanced during superheating or supercooling.
Question 10.15: Suppose that a steel of eutectoid composition is cooled to 550&deg;C (1020&deg;F) from 760&deg;C
(1400&deg;F) in less than 0.5 s and held at this temperature.
(a) How long will it take for the austenite-to-pearlite reaction to go to 50% completion? To 100% completion?
(b) Estimate the hardness of the alloy that has completely transformed to pearlite.
Solution:
We are called upon to consider the isothermal transformation of an iron-carbon alloy of eutectoid
composition.
(a) From Figure 10.22, a horizontal line at 550&deg;C intersects the 50% and reaction completion curves at
about 2.5 and 6 seconds, respectively; these are the times asked for in the problem statement.
(b) The pearlite formed will be fine pearlite. From Figure 10.30a, the hardness of an alloy of composition
0.76 wt% C that consists of fine pearlite is about 265 HB (27 HRC).
Question 10.16: Briefly cite the differences between pearlite, bainite, and spheroidite relative to
microstructure and mechanical properties.
Solution:
The microstructures of pearlite, bainite, and spheroidite all consist of α-ferrite and cementite phases. For
pearlite, the two phases exist as layers which alternate with one another. Bainite consists of very fine and parallel
needle-shaped particles of cementite that are surrounded an α-ferrite matrix. For spheroidite, the matrix is ferrite,
and the cementite phase is in the shape of sphere-shaped particles.
Bainite is harder and stronger than pearlite, which, in turn, is harder and stronger than spheroidite.
Question 10.17: What is the driving force for the formation of spheroidite?
Solution:
The driving force for the formation of spheroidite is the net reduction in ferrite-cementite phase boundary area.
Question 10.18: Using the isothermal transformation diagram for an iron–carbon alloy of eutectoid
composition (Figure 10.22), specify the nature of the final microstructure (in terms of microconstituents
present and approximate percentages of each) of a small specimen that has been subjected to the following
time–temperature treatments. In each case assume that the specimen begins at 760&deg;C (1400&deg;F) and that it has
been held at this temperature long enough to have achieved a complete and homogeneous austenitic
structure.
(a) Cool rapidly to 700&deg;C (1290&deg;F), hold for 104 s, then quench to room temperature.
Solution:
Below is Figure 10.22 upon which is superimposed the above heat treatment.
After cooling and holding at 700&deg;C for 104 s, approximately 50% of the specimen has transformed to
coarse pearlite. Upon cooling to room temperature, the remaining 50% transforms to martensite. Hence, the final
microstructure consists of about 50% coarse pearlite and 50% martensite.
(b) Reheat the specimen in part (a) to 700&deg;C (1290&deg;F) for 20 h.
Solution:
Heating to 700&deg;C for 20 h the specimen in part (a) will transform the coarse pearlite and martensite to
spheroidite.
(c) Rapidly cool to 600&deg;C (1110&deg;F), hold for 4 s, rapidly cool to 450&deg;C (840&deg;F), hold for 10 s, then quench to
room temperature.
Solution:
Below is Figure 10.22 upon which is superimposed the above heat treatment.
After cooling to and holding at 600&deg;C for 4 s, approximately 50% of the specimen has transformed to
pearlite (medium). During the rapid cooling to 450&deg;C no transformations occur. At 450&deg;C we start timing again at
zero time; while holding at 450&deg;C for 10 s, approximately 50 percent of the remaining unreacted 50% (or 25% of
the original specimen) will transform to bainite. And upon cooling to room temperature, the remaining 25% of the
original specimen transforms to martensite.
Hence, the final microstructure consists of about 50% pearlite
(medium), 25% bainite, and 25% martensite.
(d) Cool rapidly to 400&deg;C (750&deg;F), hold for 2 s, then quench to room temperature.
Solution:
Below is Figure 10.22 upon which is superimposed the above heat treatment.
After cooling to and holding at 400&deg;C for 2 s, no of the transformation begin lines have been crossed, and
therefore, the specimen is 100% austenite.
Upon cooling rapidly to room temperature, all of the specimen
transforms to martensite, such that the final microstructure is 100% martensite.
(e) Cool rapidly to 400&deg;C (750&deg;F), hold for 20 s, then quench to room temperature.
Solution:
Below is Figure 10.22 upon which is superimposed the above heat treatment.
After cooling and holding at 400&deg;C for 20 s, approximately 40% of the specimen has transformed to
bainite.
Upon cooling to room temperature, the remaining 60% transforms to martensite.
microstructure consists of about 40% bainite and 60% martensite.
(f) Cool rapidly to 400&deg;C (750&deg;F), hold for 200 s, then quench to room temperature.
Solution:
Below is Figure 10.22 upon which is superimposed the above heat treatment.
Hence, the final
After cooling and holding at 400&deg;C for 200 s, the entire specimen has transformed to bainite. Therefore,
during the cooling to room temperature no additional transformations will occur. Hence, the final microstructure
consists of 100% bainite.
(g) Rapidly cool to 575&deg;C (1065&deg;F), hold for 20 s, rapidly cool to 350&deg;C (660&deg;F), hold for 100 s, then quench to
room temperature.
Solution:
Below is Figure 10.22 upon which is superimposed the above heat treatment.
After cooling and holding at 575&deg;C for 20 s, the entire specimen has transformed to fine pearlite. Therefore,
during the second heat treatment at 350&deg;C no additional transformations will occur. Hence, the final microstructure
consists of 100% fine pearlite.
(h) Rapidly cool to 250&deg;C (480&deg;F), hold for 100 s, then quench to room temperature in water. Reheat to 315&deg;C
(600&deg;F) for 1 h and slowly cool to room temperature.
Solution:
Below is Figure 10.22 upon which is superimposed the above heat treatment.
After cooling and holding at 250&deg;C for 100 s, no transformations will have occurred—at this point, the
entire specimen is still austenite. Upon rapidly cooling to room temperature in water, the specimen will completely
transform to martensite. The second heat treatment (at 315&deg;C for 1 h)—not shown on the above plot—will
transform the material to tempered martensite. Hence, the final microstructure is 100% tempered martensite.
Question 10.20: Using the isothermal transformation diagram for a 0.45 wt% C steel alloy (Figure 10.39),
determine the final microstructure (in terms of just the microconstituents present) of a small specimen that
has been subjected to the following time-temperature treatments. In each case assume that the specimen
begins at 845&deg;C (1550&deg;F), and that it has been held at this temperature long enough to have achieved a
complete and homogeneous austenitic structure.
(a) Rapidly cool to 250&deg;C (480&deg;F), hold for 103 s, then quench to room temperature.
Solution:
Below is Figure 10.39 upon which is superimposed the above heat treatment.
While rapidly cooling to 250&deg;C about 80% of the specimen transforms to martensite; during the 1000 s
isothermal treatment at 250&deg;C no additional transformations occur. During the final cooling to room temperature,
the untransformed austenite also transforms to martensite. Hence, the final microstructure consists of 100%
martensite.
(b) Rapidly cool to 700&deg;C (1290&deg;F), hold for 30 s, then quench to room temperature.
Solution:
Below is Figure 10.39 upon which is superimposed the above heat treatment.
After cooling to and holding at 700&deg;C for 30 s, a portion of specimen has transformed to proeutectoid
ferrite. While cooling to room temperature, the remainder of the specimen transforms to martensite. Hence, the final
microstructure consists proeutectoid ferrite and martensite.
(c) Rapidly cool to 400&deg;C (750&deg;F), hold for 500 s, then quench to room temperature.
Solution:
Below is Figure 10.39 upon which is superimposed the above heat treatment.
After cooling to and holding at 400&deg;C for 500 s, all of the specimen has transformed to bainite. Hence, the
final microstructure consists of 100% bainite.
(d) Rapidly cool to 700&deg;C (1290&deg;F), hold at this temperature for 105 s, then quench to room temperature.
Solution:
Below is Figure 10.39 upon which is superimposed the above heat treatment.
After cooling to and while holding at 700&deg;C the specimen first transforms to proeutectoid ferrite and coarse
pearlite. Continued heat treating at 700&deg;C for 105 s results in a further transformation into spheroidite. Hence, the
final microstructure consists of 100% spheroidite.
(e) Rapidly cool to 650&deg;C (1200&deg;F), hold at this temperature for 3 s, rapidly cool to 400&deg;C (750&deg;F), hold for 10
s, then quench to room temperature.
Solution:
Below is Figure 10.39 upon which is superimposed the above heat treatment.
After cooling to and holding at 650&deg;C for 3 s, some of the specimen first transformers to proeutectoid
ferrite and then to pearlite (medium). During the second stage of the heat treatment at 400&deg;C, some (but not all) of
the remaining unreacted austenite transforms to bainite. As a result of the final quenching, all of the remaining
austenite transforms to martensite. Hence, the final microstructure consists of ferrite, pearlite (medium), bainite, and
martensite.
(f) Rapidly cool to 450&deg;C (840&deg;F), hold for 10 s, then quench to room temperature.
Solution:
Below is Figure 10.39 upon which is superimposed the above heat treatment.
After cooling to and holding at 450&deg;C for 10 s, a portion of the specimen first transformers to bainite.
During the quenching to room temperature, the remainder of the specimen transforms to martensite. Hence, the final
microstructure consists of bainite and martensite.
(g) Rapidly cool to 625&deg;C (1155&deg;F), hold for 1 s, then quench to room temperature.
Solution:
Below is Figure 10.39 upon which is superimposed the above heat treatment.
After cooling to and holding at 625&deg;C for 1 s, a portion of the specimen first transformers to proeutectoid
ferrite and pearlite. During the quenching to room temperature, the remainder of the specimen transforms to
martensite. Hence, the final microstructure consists of ferrite, pearlite, and martensite.
(h) Rapidly cool to 625&deg;C (1155&deg;F), hold at this temperature for 10 s, rapidly cool to 400&deg;C (750&deg;F), hold at
this temperature for 5 s, then quench to room temperature.
Solution:
Below is Figure 10.39 upon which is superimposed the above heat treatment.
After cooling to and holding at 625&deg;C for 10 s, all of the specimen transformers to proeutectoid ferrite and
pearlite. During the second part of the heat treatment at 400&deg;C no additional transformation will occur. Hence, the
final microstructure consists of ferrite and pearlite.
Question 10.23: Name the microstructural products of eutectoid iron–carbon alloy (0.76 wt% C) specimens
that are first completely transformed to austenite, then cooled to room temperature at the following rates:
(a) 200&deg;C/s,
(b) 100&deg;C/s, and
(c) 20&deg;C/s.
Solution:
We are called upon to name the microstructural products that form for specimens of an iron-carbon alloy of
eutectoid composition that are continuously cooled to room temperature at a variety of rates. Figure 10.27 is used in
these determinations.
(a) At a rate of 200&deg;C/s, only martensite forms.
(b) At a rate of 100&deg;C/s, both martensite and pearlite form.
(c) At a rate of 20&deg;C/s, only fine pearlite forms.
Question 10.24: Figure 10.40 shows the continuous cooling transformation diagram for a 1.13 wt% C ironcarbon alloy. Make a copy of this figure and then sketch and label continuous cooling curves to yield the
following microstructures:
(a) Fine pearlite and proeutectoid cementite
(b) Martensite
(c) Martensite and proeutectoid cementite
(d) Coarse pearlite and proeutectoid cementite
(e) Martensite, fine pearlite, and proeutectoid cementite
Solution:
Below is shown a continuous cooling transformation diagram for a 1.13 wt% C iron-carbon alloy, with
continuous cooling paths that will produce (a) fine pearlite and proeutectoid cementite; (b) martensite; (c)
martensite and proeutectoid cementite; (d) coarse pearlite and proeutectoid cementite; and (e) martensite, fine
pearlite, and proeutectoid cementite.
Question 10.28: Briefly describe the simplest continuous cooling heat treatment procedure that would be
used in converting a 4340 steel from one microstructure to another.
(a) (Martensite + bainite) to (ferrite + pearlite)
(b) (Martensite + bainite) to spheroidite
(c) (Martensite + bainite) to (martensite + bainite + ferrite)
Solution:
This problem asks that we briefly describe the simplest continuous cooling heat treatment procedure that
would be used in converting a 4340 steel from one microstructure to another. Solutions to this problem require the
use of Figure 10.28.
(a) In order to convert from (martensite + bainite) to (ferrite + pearlite) it is necessary to heat above about
720&deg;C, allow complete austenitization, then cool to room temperature at a rate slower than 0.006&deg;C/s.
(b) To convert from (martensite + bainite) to spheroidite the alloy must be heated to about 700&deg;C for
several hours.
(c) In order to convert from (martensite + bainite) to (martensite + bainite + ferrite) it is necessary to heat to
above about 720&deg;C, allow complete austenitization, then cool to room temperature at a rate between 0.3&deg;C/s and
0.02&deg;C/s.
Question 10.32: Rank the following iron–carbon alloys and associated microstructures from the highest to
the lowest tensile strength:
(a) 0.25 wt%C with spheroidite,
(b) 0.25 wt%C with coarse pearlite,
(c) 0.60 wt%C with fine pearlite, and
(d) 0.60 wt%C with coarse pearlite.
Justify this ranking.
Solution:
This problem asks us to rank four iron-carbon alloys of specified composition and microstructure according
to hardness. This ranking is as follows:
0.60 wt% C, fine pearlite
0.60 wt% C, coarse pearlite
0.25 wt% C, coarse pearlite
0.25 wt% C, spheroidite
The 0.25 wt% C, coarse pearlite is stronger than the 0.25 wt% C, spheroidite since coarse pearlite is
stronger than spheroidite; the composition of the alloys is the same. The 0.60 wt% C, coarse pearlite is stronger
than the 0.25 wt% C, coarse pearlite, since increasing the carbon content increases the strength. Finally, the 0.60
wt% C, fine pearlite is stronger than the 0.60 wt% C, coarse pearlite inasmuch as the strength of fine pearlite is
greater than coarse pearlite because of the many more ferrite-cementite phase boundaries in fine pearlite.
Question 10.33: Briefly explain why the hardness of tempered martensite diminishes with tempering time (at
constant temperature) and with increasing temperature (at constant tempering time).
Solution:
This question asks for an explanation as to why the hardness of tempered martensite diminishes with
tempering time (at constant temperature) and with increasing temperature (at constant tempering time). The
hardness of tempered martensite depends on the ferrite-cementite phase boundary area;
since these phase
boundaries are barriers to dislocation motion, the greater the area the harder the alloy. The microstructure of
tempered martensite consists of small sphere-like particles of cementite embedded within a ferrite matrix. As the
size of the cementite particles increases, the phase boundary area diminishes, and the alloy becomes softer.
Therefore, with increasing tempering time, the cementite particles grow, the phase boundary area decreases, and the
hardness diminishes. As the tempering temperature is increased, the rate of cementite particle growth also increases,
and the alloy softens, again, because of the decrease in phase boundary area.
Question 10.34: Briefly describe the simplest heat treatment procedure that would be used in converting a
0.76 wt% C steel from one microstructure to the other, as follows:
(a) Spheroidite to tempered martensite
(b) Tempered martensite to pearlite
(c) Bainite to martensite
(d) Martensite to pearlite
(e) Pearlite to tempered martensite
(f) Tempered martensite to pearlite
(g) Bainite to tempered martensite
(h) Tempered martensite to spheroidite
Solution:
In this problem we are asked to describe the simplest heat treatment that would be required to convert a
eutectoid steel from one microstructure to another. Figure 10.27 is used to solve the several parts of this problem.
(a) For spheroidite to tempered martensite, austenitize at a temperature of about 760&deg;C, quench to room
temperature at a rate greater than about 140&deg;C/s, then isothermally heat at a temperature between 250 and 650&deg;C.
(b) For tempered martensite to pearlite, austenitize at a temperature of about 760&deg;C, then cool to room
temperature at a rate less than about 35&deg;C/s.
(c) For bainite to martensite, first austenitize at a temperature of about 760&deg;C, then quench to room
temperature at a rate greater than about 140&deg;C/s.
(d) For martensite to pearlite, first austenitize at a temperature of about 760&deg;C, then cool to room
temperature at a rate less than about 35&deg;C/s.
(e) For pearlite to tempered martensite, first austenitize at a temperature of about 760&deg;C, then rapidly
quench to room temperature at a rate greater than about 140&deg;C/s, then isothermally heat treat (temper) at a
temperature between 250 and 650&deg;C.
(f) For tempered martensite to pearlite, first austenitize at a temperature of about 760&deg;C, then cool to room
temperature at a rate less than about 35&deg;C/s.
(g) For bainite to tempered martensite, first austenitize at a temperature of about 760&deg;C, then rapidly
quench to room temperature at a rate greater than about 140&deg;C/s, then isothermally heat treat (temper) at a
temperature between 250 and 650&deg;C.
(h) For tempered martensite to spheroidite simply heat at about 700&deg;C for approximately 20 h.
Question 10.35: (a) Briefly describe the microstructural difference between spheroidite and tempered
martensite.
(b) Explain why tempered martensite is much harder and stronger.
Solution:
(a) Both tempered martensite and spheroidite have sphere-like cementite particles within a ferrite matrix;
however, these particles are much larger for spheroidite.
(b) Tempered martensite is harder and stronger inasmuch as there is much more ferrite-cementite phase
boundary area for the smaller particles; thus, there is greater reinforcement of the ferrite phase, and more phase
boundary barriers to dislocation motion.
____________________________________________________________________________________________